Click here to load reader

View

2Download

0

Embed Size (px)

ANALYSIS OF RIPPLING IN INCOMMENSURATE ONE-DIMENSIONAL COUPLED CHAINS

PAUL CAZEAUX∗, MITCHELL LUSKIN∗, AND ELLAD B. TADMOR†

Abstract. Graphene and other recently developed 2D materials exhibit exceptionally strong in-plane stiffness. Relaxation of few-layer structures, either free-standing or on slightly mismatched substrates occurs mostly through out-of-plane bending and the creation of large-scale ripples. In this work, we present a novel double chain model, where we allow relaxation to occur by bending of the incommensurate coupled system of chains. As we will see, this model can be seen as a new application of the well-known Frenkel-Kontorova model for a one-dimensional atomic chain lying in a periodic potential. We focus in particular on modeling and analyzing ripples occurring in ground state configurations, as well as their numerical simulation.

Key words. 2D materials, heterostructures, ripples, incommensurability, atomistic relaxation, Frenkel-Kontorova

AMS subject classifications. 65Z05, 70C20, 74E15, 70G75

Introduction. Two-dimensional layered crystals such as graphene, nature’s thin- nest elastic material, exhibit exceptionally strong in-plane stiffness but are also highly flexible with extremely low flexural rigidity compared to conventional membranes. Mono- and few-layer graphene structures display spontaneous creation of long-range ripples which have been experimentally observed either in suspended conditions [14] or supported on slightly mismatched substrates [5, 21, 24]. Ripples in graphene is a multiscale phenomenon that is expected to influence its mechanical and electronic properties [17], and inducing periodic ripples in a controlled fashion may open new perspectives, e.g., for graphene-based devices [3, 15].

Various mechanisms have been described as responsible for the appearance of ripples in two-dimensional materials. Spontaneous ripples in suspended graphene monolayers have been attributed to thermal fluctuations [8] or stress [3]. Graphene monolayers supported by an almost-commensurate substrate relax to form a periodic vertical corrugation pattern [5, 18, 24, 23]. Sharp out-of-plane folds called ripplo- cations have been predicted in van der Waals (vdW) homostructures such as MoS2 multilayers, similar to line defects [13]. In a ripplocation, an additional local line of atoms is inserted in one layer leading to the formation of an out-of-plane wrinkle, while the other layer remains flat.

In this paper, we will study a different mechanism yet, where the spontaneous atomic-scale relaxation of free-standing systems of incommensurate vdW bilayers leads to a simultaneous long-range rippling of the bilayer system [19]. Note that vdW multi-layer structures tend to form naturally incommensurate stackings, either due to a relative rotation of the crystalline orientations or to a natural mismatch between the respective lattice constants. To model mathematically this multiscale phenomenon, we present a new double chain model, where we allow relaxation to occur by bending of the incommensurate coupled system of chains, as shown in Fig- ure 1. We focus in particular on modeling and analyzing rigorously ripples occurring in ground state configurations, as well as their numerical simulation. Our model was

∗School of Mathematics, University of Minnesota, Minneapolis, MN 55455 ([email protected], [email protected]) †Department of Aerospace Engineering and Mechanics, University of Minnesota, Minneapolis,

MN 55455 ([email protected])

1

ar X

iv :1

60 6.

02 61

9v 1

[ m

at h.

N A

] 8

J un

2 01

6

mailto:[email protected] mailto:[email protected] mailto:[email protected]

Fig. 1: Numerical relaxation of coupled chains by the creation of ripples.

motivated in part by the related continuum model of Nikiforov and Tadmor [19]. The model (2.6)–(2.8) developed in this work can be seen as a new application of

the well-known Frenkel-Kontorova model for a one-dimensional atomic chain lying in an incommensurate periodic potential [1, 2, 6, 4]. The role of the periodic potential is here assumed by the local interlayer contribution to the interaction energy, which is influenced by the local atom stacking configuration of the bilayer. Indeed, staggered atoms (maximizing the number of neighbors) minimize the energy compared to locally aligned configurations as seen on Figure 2 (see Section 1 for details). We will show how, by taking on some bending strain, the bilayer system is able to significantly reduce its energy by maximizing the area of staggered configurations.

Let us note that it is not possible for perfectly inextensible 2D sheets to be curved in more than one direction. As a result, a reasonable 2-dimensional model for the rippling of incommensurate layers should account for the slight extensibility of the individual layers. Thus, many simplifications used in this work, such as Eq. (2.3), cannot be used outside of our one-dimensional chain toy model.

This paper is organized as follows. First, we motivate our approach by presenting a simple numerical atomistic simulation to illustrate the phenomenon and motivate our model (see also the related example in [19]). In Section 2, we introduce a math- ematical model for the rippling mechanism, and we discuss the various assumptions that allow our explicit construction. In Section 3, we recall the classical analytical results on the Frenkel-Kontorova model due to Aubry and Le Daeron [2] that al- low us to identify the ground state configurations. In Section 4, we show how the popular supercell method of approximating the incommensurate system by periodic approximations can be rigorously justified. Finally, we present in Section 5 numerical computations that illustrate and support our analytical results.

1. Motivating numerical example. We present first a simple numerical atom- istic simulation to illustrate the phenomenon. Two coupled one-dimensional chains are fitted to represent a single zigzag row of dimers in graphene [19]. Within each chain, harmonic bonds model the interaction between nearest neighbors, and a harmonic an- gular spring is centered on each atom involving its two nearest neighbors. Between the two chains, atoms interact with a long-range Lennard-Jones potential1.Throughout

1 It is common to use the Lennard-Jones potential to model the weak interlayer van der Waals interactions in 2D layered materials. It can describe the overall cohesion of the material quite well,

2

(a) Aligned atomic configuration (b) Staggered atomic configuration

Fig. 2: Local atomic configurations: aligned situation (a) leads to a higher energy contribution than the staggered configuration (b).

this section, we work in Lennard-Jones units: � = 2.39 meV is the unit of energy and σ = 3.41 Å is the unit of length for graphene-graphene interaction, see [9].

To simulate an incommensurate system, we create a periodic supercell by choosing the equilibrium length to be slightly different in each chain: we take N1 = 232 and N2 = 233 atoms respectively in each chain for a total length of 116 σ. Periodic boundary conditions are applied at the ends. Numerical parameters are fitted to match a zigzag row of dimers in graphene [12, 19], leading to the parameterization given in Table 1.

Table 1: Numerical parameters for the atomistic simulations.

Graphene Row width Young modulus Bending modulus d = 2.13 Å Y = 21.5 eV/Å2 D = 1.46 eV

Eq. bond length Bond springs Angular springs Chain 1 l1 = 0.5 σ k1 = 130600 �/σ

2 kθ,1 = 764 � Chain 2 l2 ≈ 0.498 σ k2 ≈ 130039 �/σ2 kθ,2 ≈ 761 �

Note that the bond and angular spring constants k and kθ for each chain are related to the Young modulus Y and bending modulus D of graphene as

k = d

l Y, kθ =

d

l D,

where d is the width of the dimer row and l the equilibrium length of the bonds in the atomistic chain. In the initial configuration, each chain is in its isolated equilibrium state, and their relative distance is chosen as h = 1.063 σ. The total energy of the system is a function of all atomic positions R1i , i = 1, . . . , N1 (bottom chain) and R

2 j ,

i = 1, . . . , N2 (top chain) and also on the periodic cell length L, and can be divided into three components:

(1.1) Utot = U 1 intra + U

2 intra + Uinter.

however, it is also too smooth to correctly describe energy variations between different stacking configurations. Truly realistic computations should thus use a more accurate potential, such as the graphitic disregistry-dependent potential developed by Kolmogorov and Crespi [11]. For simplicity, and without loss of generality, we will use in this paper the Lennard-Jones potential, acknowledging that this actually leads to underestimating the formation of ripples.

3

The intralayer energies U1intra, U 2 intra take the form

(1.2)

Uνintra = 1

2

Nl∑ i=1

kν ( ‖Rνi+1 −Rνi ‖ − lν

)2 +

1

2

Nν∑ i=1

kθ,ν

( sin−1det

[ Rνi+1 −Rνi ‖Rνi+1 −Rνi ‖

, Rνi−1 −Rνi ‖Rνi−1 −Rνi ‖

])2 , ν = 1, 2,

where it is understood that periodic boundary conditions are applied: R10, R 1 N1+1

, etc. refer to the appropriate atomic position in the adjacent periodic images. The interlayer energy Uinter is

(1.3) Uinter =

N1∑ i=1

∑ j

4�

( σ ‖R2j −R1i ‖

)12 − (

σ

‖R2j −R1i ‖

)6 , where the inner sum runs over